Solution-processed amorphous gallium-tin oxide ... Solution-processed amorphous gallium-tin oxide...
Embed Size (px)
Transcript of Solution-processed amorphous gallium-tin oxide ... Solution-processed amorphous gallium-tin oxide...
mater.scichina.com link.springer.com Published online 26 December 2018 | https://doi.org/10.1007/s40843-018-9380-8 Sci China Mater 2019, 62(6): 803–812
Solution-processed amorphous gallium-tin oxide thin film for low-voltage, high-performance transistors Jinhua Ren, Kaiwen Li, Jianwen Yang, Dong Lin, Haoqing Kang, Jingjing Shao, Ruofan Fu and Qun Zhang*
ABSTRACT Gallium-tin oxide (GTO) semiconductor thin films were prepared by spin-coating with 2-methoxyethanol as the solvent. Their crystal structures, optical transparency, chemical states and surface morphologies, along with the electrical properties, were dependent on Ga contents and annealing temperatures. The optimized GTO channel layer was applied in the high-kAl2O3 thin film transistor (TFT) with a low operation voltage of 2 V, a maximum field-effect mobility of 69 cm2 V−1 s−1, a subthreshold swing (SS) of 76 mV dec−1, a threshold voltage of 0.67 V and an on-off current ratio of 1.8×107. The solution-processed amorphous- GTO-TFTs would promote the development of low-consump- tion, low-cost and high performance In-free TFT devices.
Keywords: GTO semiconductor films, thin-film transistor, sta- bility, Al2O3 dielectric
INTRODUCTION Amorphous oxide semiconductors (AOS) are achieving attention over amorphous silicon and low-temperature polycrystalline silicon (LTPS) recently . In2O3, ZnO and SnO2 based semiconductors are promising candidates for information displays [2–4]. Particularly, mass production of amorphous-InGaZnO (a-IGZO) panel has been realized. However, In is a rare element (0.25 ppm) in the earth’s upper continental crust, prompting research- ers to exploit In-free materials . As for Zn-Sn-O (ZTO)  and ZnON , weak Zn–O bonds in their lattice lead to instable thin film transistor (TFT) devices . Hence, SnO2 based semiconductors are emerging as promising channel materials. In the SnO2-based channels, Sn
4+ with a 4d105s0 electronic configuration can contribute to the high mobility, which is similar to the 5s orbital of In3+
(IGZO) . In3+ may be replaced by Sn4+ in TFTs to avoid
high fabrication cost. In the last few years, Yang et al. [10–12] prepared high performance SnO2-based TFTs by radio-frequency (RF) magnetron sputtering. It is well known that ion bombardment and incorporation results in a large number of defects in the films . In addition, in the sputtering process, multi-metal thin film probably has different composition from the target due to preferential sputtering, especially for IGZO . There- fore, more researchers are turning to solution process method for realizing low-cost electronics. Recent reports [15,16] showed solution processed SnO2 TFTs have better performance than vacuum based devices. Pure SnO2 films tend to crystallize, which does not lead to the uniformity for TFT devices. Besides, high carrier concentration in pure SnO2 also affects the electrical performance of devices, such as stability and current on-off ratio (Ion/Ioff). From the periodic table of elements, it can be found that the similar ion radius of Ga (0.62 Å) and Sn (0.69 Å) may reduce structural defects in the Ga-doped SnO2 system. In the previous reports [17,18], Ga is an oxygen vacancy inhibitor and can weaken the crystallinity of films. Recently, Matsuda et al.  reported RF magnetron sputtered a-GaSnO (GTO)-TFTs with high mobility of 25.6 cm2 V−1 s−1 at 350°C. Zhang et al.  reported nanocrystalline Ga-rich GTO-TFTs with mobility of 1.03 cm2 V−1 s−1 at 900°C. The high annealing tempera- ture is not compatible with high-k dielectric and flexible substrates. In this paper, solution-processed a-GTO-TFTs with
various Ga content and under different annealing temperatures are investigated. The stability of the optimum device is evaluated. Based on these results, a-GTO-TFTs with Al2O3 high-k dielectric layer show high mobility and low operation voltage.
Department of Materials Science, National Engineering Laboratory for TFT-LCD Materials and Technologies, Fudan University, Shanghai 200433, China * Corresponding author (email: firstname.lastname@example.org)
SCIENCE CHINA Materials. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .ARTICLES
June 2019 | Vol. 62 No.6 803© Science China Press and Springer-Verlag GmbH Germany, part of Springer Nature 2018
http://mater.scichina.com http://link.springer.com https://doi.org/10.1007/s40843-018-9380-8 http://crossmark.crossref.org/dialog/?doi=10.1007/s40843-018-9380-8&domain=pdf&date_stamp=2018-12-13
Precursor solution preparation 0.1 mol L−1 SnCl2·2H2O (Aladdin, 99.99%) and various amounts of Ga(NO3)3·xH2O (Aladdin, 99.9%) (Ga:Sn = 0, 10, 20, 50 at.%) were dissolved in 10 mL 2-methox- yethanol successively in sealed reagent bottles. Then, they were stirred by a magnetic stirrer at room temperature for 2 h in ambient. For Al2O3 dielectric, 0.3 mol L
Al(NO3)3·9H2O (Aladdin, 99.99%) was dissolved in 5 mL 2-methoxyethanol and then stirred at room temperature for 3 h.
Thin film and device fabrication For GTO-SiO2 device, p-Si with 270 nm thermally grown SiO2 was cleaned by acetone, ethyl alcohol and deionized water successively. Then the surface of SiO2 was treated by oxygen plasma to improve the adhesive strength of GTO solution. The above GTO solutions were filtered through 0.22 μm PTFE filter and then spin-coated onto the SiO2 substrate with the rotation speed of 3,500 rpm for 30 s. The sol films were then baked on a hot plate to be preheated at 150°C for 10 min to evaporate the solvent. The resulting gel films were annealed in a tube furnace at 300, 350 and 400°C for 1 h in air. Finally, ITO source/ drain (S/D) electrode arrays (W/L=450 μm/80 μm,W and L is width and length of electrodes) were deposited by RF magnetron sputtering. For GTO-Al2O3 device, p-Si wafers were ultrasonically cleaned by 2% HF aqueous solution, water, acetone and ethyl alcohol. Similarly, they were bombarded with oxygen plasma to improve hydrophili- city. The prepared Al3+ solution was also filtered through 0.22 μm PTFE filter and spun onto the Si wafers. Then, it was pre-annealed on a hotplate at 220°C for 10 min. The samples were then cured under ultraviolet lamp for 10 min to promote the crosslinking reactions in the gel film. Taking the annealing temperature of active layers into account, the cured Al2O3 gel films were then annealed at 450°C in air for 30 min. The fabrication method of channel layers is similar to the GTO-SiO2 device. The entire device was completed after the deposition of ITO electrodes. In the meantime, the GTO films were also spin-coated on a glass substrate under the same condition.
Thin film and device characterization The thermal behavior of GTO and Al2O3 precursor solutions was monitored in ambient air using a thermal gravimetric (TGA, TA Q500) with a heating rate of 10°C min−1. The film thicknesses were measured via a
stylus profiler (Kosaka Laboratory ET3000). The device structure was observed by a field-emission scanning electron microscope (FE-SEM-4800-1) in sectional view. The surface information of thin films was detected by energy disperse spectroscopy (EDS) attachment. X-ray diffraction (XRD, Bruker D8 Advanced and Da Vinci Design system) was used to characterize the crystal structure of thin films. Optical transmittance of GTO films was obtained from ultraviolet-visible (UV, Shimad- zu, UV2400) spectrophotometer. X-ray photoelectron spectroscopy (XPS, ThermoFischer, ESCALAB 250Xi) was used to analyze the chemical components and oxidation states of the surfaces of GTO channels. The surface morphologies of active layer were examined by an atomic force microscope (AFM, Dimension Edge, Bruker). The capacitance per unit area of Al2O3 dielectric layer was measured with a WK6515B precision impedance analyzer. I–V, transfer and output character- istic curves of GTO-TFTs were measured by a Keithley 4200 semiconductor parameter analyzer.
RESULTS AND DISCUSSION Fig. 1a shows the TGA curves of Al2O3 and 20 at.% GTO gels where the initial weight loss below 130°C is due to the evaporation of 2-methoxyethanol (gray region). The gradual weight loss up to 400°C for Al2O3 gel is ascribed to the evaporation of the bound water and the decomposition of nitrate groups (yellow region) . For GTO gel, condensation process gradually leads to a network of Ga–Sn–O bonds with increasing temperature (yellow region) . The faster mass loss for Al2O3 gel may originate from the lower Al3+ weight ratio in the Al2O3 precursor solution (7.2 wt.%) than that of GTO solution (52.6 wt.% for Sn4+, 27.3 wt.% for Ga3+). Fig. 1b shows the XRD patterns of GTO thin films on glass substrates annealed at 350°C with Ga content from 0 to 50 at.%. The pure SnO2 film shows a weak peak at 2θ=37.9°, representing (200) crystal planes of cassiterite SnO2 (JCPDS No. 41-1445) . The poor crystallinity may be due to a low temperature. It is reported that SnO2 films present obvious polycrystalline peaks at the temperature above 350°C . However, the unobvious peak after doping 10 at.% Ga indicates that Ga can inhibit the crystallization of SnO2 lattice. As the Ga content increases to 20 and 50 at.%, GTO thin film becomes amorphous. The degradation of SnO2 thin film crystal- linity may derive from the induced stress and the distortion of structures . Due to ionic radius difference, Ga3+ may occupy Sn4+ sites in GTO films. Optical spectra of GTO films demonstrate the transmit-
ARTICLES . . . . . . . . . . . . . . . . . . . . . . . . . SCIENCE CHINA Materials
804 June 2019 | Vol. 62 No.6© Science China Press and Springer-Verlag GmbH Germany, part of Springer Nature 2018
tance more than 95% from 400 to 700